Thermoplastic elastomers (TPE), sometimes referred to as thermoplastic rubbers, are a class of copolymers or a physical mix of polymers (usually a plastic and a rubber) which consist of materials with both thermoplastic and elastomeric properties. While most elastomers are thermosets, thermoplastics are in contrast relatively easy to use in manufacturing, for example, by injection molding. Thermoplastic elastomers show advantages typical of both rubbery materials and plastic materials. The principal difference between thermoset elastomers and thermoplastic elastomers is the type of crosslinking bond in their structures. In fact, crosslinking is a critical structural factor which contributes to impart high elastic properties.
There are six generic classes of commercial TPEs:
- Styrenic block copolymers (TPE-s)
- Polyolefin blends (TPE-o)
- Elastomeric alloys (TPE-v or TPV)
- Thermoplastic polyurethanes (TPU)
- Thermoplastic copolyester
- Thermoplastic polyamides.
Examples of TPE products that come from block copolymers group are Arnitel (DSM), Solprene (Dynasol), Engage (Dow Chemical), Hytrel (Du Pont), Dryflex and Mediprene (ELASTO), Kraton (Kraton Polymers), Pibiflex. Example of TPV is FORPRENE. Examples of Styrenic block copolymers (TPE-s) are SOFPRENE (SBS) and LAPRENE (SEBS). In order to qualify as a thermoplastic elastomer, a material must have these three essential characteristics:
- The ability to be stretched to moderate elongations and, upon the removal of stress, return to something close to its original shape.
- Processable as a melt at elevated temperature.
- Absence of significant creep.
It was not until the 1950s, when thermoplastic polyurethane polymers became available, that TPE became a commercial reality. During the 1960s styrene block copolymer became available, and in the 1970s a wide range of TPEs came on the scene. The worldwide usage of TPEs (680,000 tons/year in 1990) is growing at about 9% per year. The styrene-butadiene materials possess a two-phase microstructure due to incompatibility between the polystyrene and polybutadiene blocks, the former separating into spheres or rods depending on the exact composition. With low polystyrene content, the material is elastomeric with the properties of the polybutadiene predominating. Generally they offer a much wider range of properties than conventional cross-linked rubbers because the composition can vary to suit customer needs.
Block copolymers are interesting because they can "microphase separate" to form periodic nanostructures, as in the styrene-butadiene-styrene block copolymer shown at right. The polymer is known as Kraton and is used for shoe soles and adhesives. Owing to the microfine structure, the transmission electron microscope or TEM was needed to examine the structure. The butadiene matrix was stained with osmium tetroxide to provide contrast in the image. The material was made by living polymerization so that the blocks are almost monodisperse, so helping to create a very regular microstructure. The molecular weight of the polystyrene blocks in the main picture is 102,000; the inset picture has a molecular weight of 91,000, producing slightly smaller domains. The spacing between domains has been confirmed by small-angle X-ray scattering, a technique which gives information about microstructure. Since most polymers are incompatible with one another, forming a block polymer will usually result in phase separation, and the principle has been widely exploited since the introduction of the SBS block polymers, especially where one of the block is highly crystalline. One exception to the rule of incompatibility is the material Noryl, where polystyrene and polyphenylene oxide or PPO form a continuous blend with one another.
Other TPE's have crystalline domains where one kind of block co-crystallizes with other block in adjacent chains, such as in copolyester rubbers, achieving the same effect as in the SBS block polymers. Depending on the block length, the domains are generally more stable than the latter owing to the higher crystal melting point. That point determines the processing temperatures needed to shape the material, as well as the ultimate service use temperatures of the product. Such materials include Hytrel, a polyester-polyether copolymer and Pebax, a nylon or polyamide-polyether copolymer.
TPE materials have the potential to be recyclable since they can be molded, extruded and reused like plastics, but they have typical elastic properties of rubbers which are not recyclable owing to their thermosetting characteristics. TPE also require little or no compounding, with no need to add reinforcing agents, stabilizers or cure systems. Hence, batch-to-batch variations in weighting and metering components are absent, leading to improved consistency in both raw materials and fabricated articles. TPEs can be easily colored by most types of dyes. Besides that, it consumes less energy and closer and more economical control of product quality is possible.
The two most important manufacturing methods with TPEs are extrusion and injection molding. Compression molding is seldom, if ever, used. Fabrication via injection molding is extremely rapid and highly economical. Both the equipment and methods normally used for the extrusion or injection molding of a conventional thermoplastic are generally suitable for TPEs. TPEs can also be processed by blow molding, thermoforming, and heat welding.
TPEs are used where conventional elastomers cannot provide the range of physical properties needed in the product. These materials find large application in the automotive sector and in household appliances sector. Thus copolyester TPEs are used in snowmobile tracks where stiffness and abrasion resistance are at a premium. They are also widely used for catheters where nylon block copolymers offer a range of softness ideal for patients. Thermoplastic silicon and olefin blends are used for extrusion of glass run and dynamic weatherstripping car profiles. Styrene block copolymers are used in shoe soles for their ease of processing, and widely as adhesives. TPE is commonly used to make suspension bushings for automotive performance applications because of its greater resistance to deformation when compared to regular rubber bushings. TPE may also be used in products meant for bodily insertion, such as menstrual cups, and sex toys. TPE is also finding more and more uses as an electrical cable jacket/inner insulation. TPE is also used in some headphone cables.
- PR Lewis and C Price, Polymer, 13, 22 (1972)
- Modern Plastic Mid-October Encyclopedia Issue, Introduction to TPEs, page:109-110
- "Definitions of terms relating to the structure and processing of sols, gels, networks, and inorganic-organic hybrid materials (IUPAC Recommendations 2007)". Pure and Applied Chemistry 79 (10): 1801–1829. 2007. doi:10.1351/pac200779101801.
- "MeLuna Classic Menstrual Cup". Retrieved August 15, 2012.
- "Fill-er-Up Butt Plug Kit". Retrieved August 15, 2012.
||This article may contain promotional material and other spam. (November 2010)|